- Nano Express
- Open Access

# Tuning electronic and magnetic properties of partially hydrogenated graphene by biaxial tensile strain: a computational study

- Er Hong Song
^{1}, - Ghafar Ali
^{1}, - Sung Ho Yoo
^{1}, - Qing Jiang
^{2}and - Sung Oh Cho
^{1}Email author

**9**:491

https://doi.org/10.1186/1556-276X-9-491

© Song et al.; licensee Springer. 2014

**Received:**14 August 2014**Accepted:**5 September 2014**Published:**13 September 2014

## Abstract

Using density functional theory calculations, we have investigated the effects of biaxial tensile strain on the electronic and magnetic properties of partially hydrogenated graphene (PHG) structures. Our study demonstrates that PHG configuration with hexagon vacancies is more energetically favorable than several other types of PHG configurations. In addition, an appropriate biaxial tensile strain can effectively tune the band gap and magnetism of the hydrogenated graphene. The band gap and magnetism of such configurations can be continuously increased when the magnitude of the biaxial tensile strain is increased. This fact that both the band gap and magnetism of partially hydrogenated graphene can be tuned by applying biaxial tensile strain provides a new pathway for the applications of graphene to electronics and photonics.

## Keywords

- Graphene
- Band gap
- Magnetism
- Strain

## Background

Graphene has recently attracted considerable attention owing to its remarkable electronic and structural properties in many emerging application areas such as electronic devices [1–3]. However, graphene exhibits a zero band gap and nonmagnetic behavior, which limits its application in electronics and photonics [4]. Earlier investigations, both theoretically [5–33] and experimentally [34–43], have been made to adjust electronic and magnetic properties of graphene. There are two basic mechanisms cataloged among these schemes, either to disturb the band crossing at Dirac points via breaking the equivalence of the two sublattices of graphene or to transform the carbon hybridization from sp^{2} into sp^{3} via chemical functionalization.

The first mechanism can be achieved by substrate-graphene interaction [5, 6, 35], applying external electric field [36, 37], uniaxial strain [7, 8], cutting graphene into nanoribbons [9–11, 38] and adsorption of molecules on graphene surface [12–14]. However, the efforts of the abovementioned approaches are limited and can only open a tiny band gap because of the robust π bands of graphene. Another mechanism can be realized via chemical functionalization of graphene, such as H, F, OH, COOH, and O chemisorbed on either one side or both sides of graphene [15–23]. At present, this approach can induce a large band gap opening of graphene: for example, fully hydrogenated graphene has been shown to be a wide band gap semiconductor [16], whereas half-hydrogenated graphene results in an indirect gap and ferromagnetism [26].

Motivated by the above results, we have carried out a systematic investigation to explore the stability and electronic and magnetic properties of partially hydrogenated graphene (PHG) by applying biaxial tensile strain using density functional theory. The calculated results indicate that the configuration with removing H-hexagon is the most energetically favorable in several types of HG configurations, while the appropriate biaxial tensile strain can effectively tune the band gap and magnetism of the partially hydrogenated graphene.

## Methods

All calculations in this study were performed using the spin-polarized first-principle method as implemented in the DMol^{3} code [44]. The generalized gradient approximation (GGA) with the Perdew-Burke-Ernzerhof (PBE) exchange-correlation functional was used [45], in combination with the double numerical plus polarization (DNP). The empirically corrected density functional theory (DFT + D) method within the Grimme scheme was employed in all the calculations to consider the van der Waals forces [46]. All-electron core treatment was adopted, and the real space global cutoff radius was set to be 4.6 Å to achieve high accuracy. We used the smearing techniques with a smearing value of 0.005 Ha.

^{−5}hartree, and that of maximum force in 0.002 hartree. The stability of hydrogenated graphene was determined from the formation energy

*E*

_{f}by the following:

where *E*_{total}(*n*) is the cohesive energy of the system, *n* was the number of H atoms removed from a graphane sheet, and μ_{H} (μ_{graphane}) is the chemical potential of the constituent H (graphane) at a given state. Here, we chose the binding energy per atom of H_{2} molecule as μ_{H}. And μ_{graphane} was taken as the cohesive energy of a single graphane sheet.

## Results and discussion

According to the previous reports [16, 47], two favorable structures of fully hydrogenated graphene (graphene), chair and boat conformations, exist. In the chair configuration, every two adjacent C atoms are hydrogenated from the opposite sides of the graphene sheet. The induced strains compensate each other and thereby the energy of graphane is low. While in the boat conformation, H atoms are alternately bonded to C atoms on both sides in pairs. Due to the repulsion of two neighboring H on the same side, the boat configuration is less stable than the chair one. Therefore, we only consider the chair configuration. For the case of graphane, the obtained lattice parameter, C-C bond length, and C-H bond length of graphane are 2.54, 1.54, and 1.11 Å, respectively, which are in good agreement with previous reported data [25].

*E*

_{f}of the H vacancies on graphane can be calculated from the difference between the total energy of graphane and the sum of the total energy of dehydrogenated graphane and those of detached single H atoms. In Equation (1), positive

*E*

_{f}represents endothermic process of dehydrogenation. The calculations show that

*E*

_{f}of paired vacancies is always smaller than that of two unpaired vacancies (Figure 1a,b,c). In other words, paired vacancies are more easily formed than unpaired vacancies in graphane. This can be explained by the fact that a single H vacancy creates a dangling bond and raises the total energy due to a local strain [23]. In the condition of paired dehydrogenation, both unsaturated C atoms are turned to sp

^{2}hybridized state and form a C = C double bond, through which the two π electrons pair together and the vacancy-induced local strain can be partially released. The removal of radicals by C = C double bond has significant effect on the electronic structures of the dehydrogenated graphane. As shown in Figure 1d,e,f,g,h,i, three adjacent paired vacancies formed a hexagon vacancy and graphane with a hexagon vacancy is more energetically favorable than five separated paired vacancies.

*E*

_{g}) of the perfect graphane is about 4.41 eV. The

*E*

_{g}opening in graphene can be attributed to the changes of functionalized C atoms from sp

^{2}to sp

^{3}hybridization. However, after partially dehydrogenation of graphane, the

*E*

_{g}and the corresponding electronic structures can be changed. According to the unified geometric rule reported by previous works [48, 49], the spin state at all zigzag edges with angles of either 0° or 120° between the edges should be ferromagnetic (FM), whereas it should be antiferromagnetic (AFM) if the edges are aligned at angles of 60° and 180° with respect to each other. On the basis of this rule, we calculated the band structures of C98H92 (1-hexagon vacancy, Figure 2a), C98H88 (2-hexagon vacancies, Figure 2b), C98H85 (triangle vacancy formed by 3-hexagon vacancies, Figure 2c), C98H72 (2-triangle vacancies, Figure 2d), C98H59 (3-triangle vacancies, Figure 2e), and C98H46 (4-triangle vacancies, Figure 2f) via selective dehydrogenation. As shown in Figure 3, it is found that the values of

*E*

_{g}of partially dehydrogenated graphane decrease as the hexagon vacancies increase. Thus, the insulating graphane with a wide band gap becomes a semiconductor via appropriate dehydrogenation.

*E*

_{g}of PHG which are induced by the quantum confinement effect in PHG with increased vacancies. In other words, the trend of band gap narrowing can be attributed to the number of edge states in the PHG with the hexagon vacancies [22, 49–52]. Taking the structure of C98H85 as an example, the

*E*

_{g}reduces to 0.52 eV and the magnetic moment (

*m*) is about 0.98

*μ*

_{B}(Figure 3c). When the triangle vacancies of graphane increase to four, the band structure of C98H46 has an indirect band gap with

*E*

_{g}= 0.33 eV, whereas

*m*increases to 3.90

*μ*

_{B}(Figure 3f). Meanwhile, the strong σ-bonds are broken between C and H atoms and removal of the nearest neighbor H atoms leads to C = C double bonds, leaving the electrons in the unpaired C atoms localized and unpaired. In order to study the preferred coupling of these moments, we considered the following three magnetic configurations of C98H46: FM coupling, antiferromagnetic (AF) coupling, and nonmagnetic (NM) state, where the calculation is spin unpolarized. From the calculated results, it is found that the total energy of FM state is lower than that of AF and NM states, respectively. Thus, we can deduce that the ground state is FM state.

*E*

_{g}of C98H46 increases monotonically as the increase of strain (Figure 4a), even a 1% strain, can result in a 0.02 eV gap increase. This trend is similar to the case of graphene, as Topsakal et al. demonstrated that the

*E*

_{g}of graphane monolayer increases with increasing biaxial tensile strain up to 15% [53]. The

*E*

_{g}of C98H46 system increases to 0.44 eV with tensile strain reaches 9%. Note that when the tensile strain is lower than 9%, C98H46 system is always semiconducting with an indirect band gap. As shown in Figure 4b, we next investigate the influences of tensile ϵ on the magnetic of C98H46 system. Under tensile strain ϵ, C98H46 system always keeps the FM state as in the unstrained case. As ϵ increases to 9%, it is clear that the magnetic moment of C98H46 system slowly increase to 3.94 μ

_{ B }

*.*

From the above results, we conclude that the electronic and magnetic properties of graphane can be efficiently tuned from insulator to semiconductor (from non-magnetism to ferromagnetism) via selective dehydrogenation, whereas the band gap and magnetism moment of partially hydrogenated graphene can be enhanced by imposing a biaxial tensile strain.

## Conclusions

In summary, DFT calculations with biaxial tensile strain are carried out to investigate the effects of biaxial tensile strain on the electronic and magnetic properties of PHG structures. It is found that the configuration with removing H-hexagon is the most energetically favorable in the several types of HG configurations. In addition, the appropriate biaxial tensile strain can effectively increase the band gap and magnetism of PHG. Overall, tuning both band gap and magnetism of hydrogenated graphene by applying biaxial tensile strain provides a new perspective for wide applications of graphene in electronics and photonics.

## Declarations

### Acknowledgements

This work was supported by a National Research Foundation of Korea (NRF) grant funded by the Korea government (MEST) (No. 2012–0009523).

## Authors’ Affiliations

## References

- Geim AK: Graphene: status and prospects.
*Science*2009, 324: 1530–1534. 10.1126/science.1158877View ArticleGoogle Scholar - Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films.
*Science*2004, 306: 666–669. 10.1126/science.1102896View ArticleGoogle Scholar - Huang Q, Kim JJ, Ali G, Cho SO: Width-tunable graphene nanoribbons on a SiC substrate with a controlled step height.
*Adv Mater*2013, 25: 1144–1148. 10.1002/adma.201202746View ArticleGoogle Scholar - Novoselov K: Graphene: mind the gap.
*Nat Mater*2007, 6: 720–721. 10.1038/nmat2006View ArticleGoogle Scholar - Giovannetti G, Khomyakov PA, Brocks G, Kelly PJ, van den Brink J: Substrate-induced band gap in graphene on hexagonal boron nitride: Ab initio density functional calculations.
*Phys Rev B*2007, 76: 073103.View ArticleGoogle Scholar - Chen XF, Lian JS, Jiang Q: Band-gap modulation in hydrogenated graphene/boron nitride heterostructures: the role of heterogeneous interface.
*Phys Rev B*2012, 86: 125437.View ArticleGoogle Scholar - Gui G, Li J, Zhong J: Band structure engineering of graphene by strain: first-principles calculations.
*Phys Rev B*2008, 78: 075435.View ArticleGoogle Scholar - Sun L, Li Q, Ren H, Su H, Shi QW, Yang J: Strain effect on electronic structures of graphene nanoribbons: a first-principles study.
*J Chem Phys*2008, 129: 074704. 10.1063/1.2958285View ArticleGoogle Scholar - Dai QQ, Zhu Y, Jiang Q, Dai QQ, Zhu Y, Jiang Q: Electronic and magnetic engineering in zigzag graphene nanoribbons having a topological line defect at different positions with or without strain.
*J Phys Chem C*2013, 117(9):47914799.View ArticleGoogle Scholar - Son Y-W, Cohen ML, Louie SG: Energy gaps in graphene nanoribbons.
*Phys Rev Lett*2006, 97: 216803.View ArticleGoogle Scholar - Dai QQ, Zhu YF, Jiang Q: Electronic and magnetic properties of armchair graphene nanoribbons with 558 grain boundary.
*Phys Chem Chem Phys*2014, 16: 10607–10613. 10.1039/c4cp00868eView ArticleGoogle Scholar - Lu YH, Chen W, Feng YP, He PM: Tuning the electronic structure of graphene by an organic molecule.
*J Phys Chem B*2008, 113: 2–5.View ArticleGoogle Scholar - Zanella I, Guerini S, Fagan SB, Mendes Filho J, Souza Filho AG: Chemical doping-induced gap opening and spin polarization in graphene.
*Phys Rev B*2008, 77: 073404.View ArticleGoogle Scholar - Ribeiro RM, Peres NMR, Coutinho J, Briddon PR: Inducing energy gaps in monolayer and bilayer graphene: local density approximation calculations.
*Phys Rev B*2008, 78: 075442.View ArticleGoogle Scholar - Boukhvalov DW, Katsnelson MI, Lichtenstein AI: Hydrogen on graphene: electronic structure, total energy, structural distortions and magnetism from first-principles calculations.
*Phys Rev B*2008, 77: 035427.View ArticleGoogle Scholar - Sofo JO, Chaudhari AS, Barber GD: Graphane: a two-dimensional hydrocarbon.
*Phys Rev B*2007, 75: 153401.View ArticleGoogle Scholar - Lebègue S, Klintenberg M, Eriksson O, Katsnelson MI: Accurate electronic band gap of pure and functionalized graphane from GW calculations.
*Phys Rev B*2009, 79: 245117.View ArticleGoogle Scholar - Duplock EJ, Scheffler M, Lindan PJD: Hallmark of perfect graphene.
*Phys Rev Lett*2004, 92: 225502.View ArticleGoogle Scholar - Boukhvalov DW, Katsnelson MI: Tuning the gap in bilayer graphene using chemical functionalization: density functional calculations.
*Phys Rev B*2008, 78: 085413.View ArticleGoogle Scholar - Lu N, Li Z, Yang J: Electronic structure engineering via on-plane chemical functionalization: a comparison study on two-dimensional polysilane and graphane.
*J Phys Chem C*2009, 113: 16741–16746. 10.1021/jp904208gView ArticleGoogle Scholar - Yan J-A, Xian L, Chou MY: Structural and electronic properties of oxidized graphene.
*Phys Rev Lett*2009, 103: 086802.View ArticleGoogle Scholar - Dai QQ, Zhu Y, Jiang Q: Stability, electronic and magnetic properties of embedded triangular graphene nanoflakes.
*Phys Chem Chem Phys*2012, 14: 1253–1261. 10.1039/c1cp22866hView ArticleGoogle Scholar - Gao H, Wang L, Zhao J, Ding F, Lu J: Band gap tuning of hydrogenated graphene: H coverage and configuration dependence.
*J Phys Chem C*2011, 115: 3236–3242. 10.1021/jp1094454View ArticleGoogle Scholar - Li Y, Zhou Z, Shen P, Chen Z: Structural and electronic properties of graphane nanoribbons.
*J Phys Chem C*2009, 113: 15043–15045. 10.1021/jp9053499View ArticleGoogle Scholar - Singh AK, Penev ES, Yakobson BI: Vacancy clusters in graphane as quantum dots.
*ACS Nano*2010, 4: 3510–3514. 10.1021/nn1006072View ArticleGoogle Scholar - Zhou J, Wang Q, Sun Q, Chen XS, Kawazoe Y, Jena P: Ferromagnetism in semihydrogenated graphene sheet.
*Nano Lett*2009, 9: 3867–3870. 10.1021/nl9020733View ArticleGoogle Scholar - Ribas M, Singh A, Sorokin P, Yakobson B: Patterning nanoroads and quantum dots on fluorinated graphene.
*Nano Res*2011, 4: 143–152. 10.1007/s12274-010-0084-7View ArticleGoogle Scholar - Wu M, Wu X, Zeng XC: Exploration of half metallicity in edge-modified graphene nanoribbons.
*J Phys Chem C*2010, 114: 3937–3944. 10.1021/jp100027wView ArticleGoogle Scholar - Wehling TO, Katsnelson MI, Lichtenstein AI: Impurities on graphene: midgap states and migration barriers.
*Phys Rev B*2009, 80: 085428.View ArticleGoogle Scholar - Zhu Y, Lian J, Jiang Q: Role of edge geometry and magnetic interaction in opening bandgap of Low-dimensional graphene.
*ChemPhysChem*2014, 15: 958–965. 10.1002/cphc.201301127View ArticleGoogle Scholar - Zhu Y, Zhao N, Lian J, Jiang Q: Toward tandem photovoltaic devices employing nanoarray graphene-based sheets.
*J Phys Chem C*2014, 118: 2385–2390.View ArticleGoogle Scholar - Zhu YF, Dai QQ, Zheng WT, Jiang Q: Gap openings in graphene regarding interfacial interaction from substrates.
*Phys Chem Chem Phys*2014, 16: 5600–5604. 10.1039/c3cp55222eView ArticleGoogle Scholar - Zhu YF, Dai QQ, Zhao M, Jiang Q: Physicochemical insight into gap openings in graphene.
*Sci Rep*2013., 3:Google Scholar - Jung I, Dikin DA, Piner RD, Ruoff RS: Tunable electrical conductivity of individual graphene oxide sheets reduced at “low” temperatures.
*Nano Lett*2008, 8: 4283–4287. 10.1021/nl8019938View ArticleGoogle Scholar - Zhou SY, Gweon GH, Fedorov AV, First PN, de Heer WA, Lee DH, Guinea F, Castro Neto AH, Lanzara A: Substrate-induced bandgap opening in epitaxial graphene.
*Nat Mater*2007, 6: 770–775. 10.1038/nmat2003View ArticleGoogle Scholar - Zhang Y, Tang T-T, Girit C, Hao Z, Martin MC, Zettl A, Crommie MF, Shen YR, Wang F: Direct observation of a widely tunable bandgap in bilayer graphene.
*Nature*2009, 459: 820–823. 10.1038/nature08105View ArticleGoogle Scholar - Castro EV, Novoselov KS, Morozov SV, Peres NMR, dos Santos JMBL, Nilsson J, Guinea F, Geim AK, Neto AHC: Biased bilayer graphene: semiconductor with a gap tunable by the electric field effect.
*Phys Rev Lett*2007, 99: 216802.View ArticleGoogle Scholar - Han MY, Özyilmaz B, Zhang Y, Kim P: Energy band-gap engineering of graphene nanoribbons.
*Phys Rev Lett*2007, 98: 206805.View ArticleGoogle Scholar - Wu X, Sprinkle M, Li X, Ming F, Berger C, de Heer WA: Epitaxial-graphene/graphene-oxide junction: an essential step towards epitaxial graphene electronics.
*Phys Rev Lett*2008, 101: 026801.View ArticleGoogle Scholar - Jeong HK, Jin MH, So KP, Lim SC, Lee YH: Tailoring the characteristics of graphite oxides by different oxidation times.
*J Phys D Appl Phys*2009, 42: 065418. 10.1088/0022-3727/42/6/065418View ArticleGoogle Scholar - Luo Z, Vora PM, Mele EJ, Johnson ATC, Kikkawa JM: Photoluminescence and band gap modulation in graphene oxide.
*Appl Phys Lett*2009, 94: 111909. 10.1063/1.3098358View ArticleGoogle Scholar - Balog R, Jorgensen B, Nilsson L, Andersen M, Rienks E, Bianchi M, Fanetti M, Laegsgaard E, Baraldi A, Lizzit S, Sljivancanin Z, Besenbacher F, Hammer B, Pedersen TG, Hofmann P, Hornekaer L: Bandgap opening in graphene induced by patterned hydrogen adsorption.
*Nat Mater*2010, 9: 315–319. 10.1038/nmat2710View ArticleGoogle Scholar - Elias DC, Nair RR, Mohiuddin TMG, Morozov SV, Blake P, Halsall MP, Ferrari AC, Boukhvalov DW, Katsnelson MI, Geim AK, Novoselov KS: Control of Graphene's Properties by Reversible Hydrogenation: Evidence for Graphane.
*Science*2009, 323: 610–613. 10.1126/science.1167130View ArticleGoogle Scholar - Delley B: From molecules to solids with the DMol(3) approach.
*J Chem Phys*2000, 113: 7756–7764. 10.1063/1.1316015View ArticleGoogle Scholar - Perdew JP, Burke K, Ernzerhof M: Generalized gradient approximation made simple.
*Phys Rev Lett*1996, 77: 3865–3868. 10.1103/PhysRevLett.77.3865View ArticleGoogle Scholar - Grimme S: Semiempirical GGA-type density functional constructed with a long-range dispersion correction.
*J Comput Chem*2006, 27: 1787–1799. 10.1002/jcc.20495View ArticleGoogle Scholar - Singh AK, Yakobson BI: Electronics and magnetism of patterned graphene nanoroads.
*Nano Lett*2009, 9: 1540–1543. 10.1021/nl803622cView ArticleGoogle Scholar - Yu D, Lupton E, Gao HJ, Zhang C, Liu F: A unified geometric rule for designing nanomagnetism in graphene.
*Nano Res*2008, 1: 497–501. 10.1007/s12274-008-8053-0View ArticleGoogle Scholar - Yu D, Lupton E, Liu M, Liu W, Liu F: Collective magnetic behavior of graphene nanohole superlattices.
*Nano Res*2008, 1: 56–62. 10.1007/s12274-008-8007-6View ArticleGoogle Scholar - Pedersen TG, Flindt C, Pedersen J, Mortensen NA, Jauho A-P, Pedersen K: Graphene antidot lattices: designed defects and spin qubits.
*Phys Rev Lett*2008, 100: 136804.View ArticleGoogle Scholar - Liu W, Wang ZF, Shi QW, Yang J, Liu F: Band-gap scaling of graphene nanohole superlattices.
*Phys Rev B*2009, 80: 233405.View ArticleGoogle Scholar - Park C-H, Yang L, Son Y-W, Cohen ML, Louie SG: Anisotropic behaviours of massless Dirac fermions in graphene under periodic potentials.
*Nat Phys*2008, 4: 213–217. 10.1038/nphys890View ArticleGoogle Scholar - Topsakal M, Cahangirov S, Ciraci S: The response of mechanical and electronic properties of graphane to the elastic strain.
*Appl Phys Lett*2010, 96: 091912. 10.1063/1.3353968View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.